Create Presentation
Download Presentation

Download Presentation

Hot Mix Asphalt (HMA) Volumetric Properties

Download Presentation
## Hot Mix Asphalt (HMA) Volumetric Properties

- - - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - - -

**HMA Volumetric Terms**• Bulk specific gravity (BSG) of compacted HMA • Maximum specific gravity • Air voids • Effective specific gravity of aggregate • Voids in mineral aggregate, VMA • Voids filled with asphalt, VFA**Va**VMA Vb Vba Vse Vmm Vmb Vsb Volumetric Relationships**Mass agg. and AC**Vol. agg., AC, air voids Gmb = BSG of Compacted HMA • AC mixed with agg. and compacted into sample**Testing**• Mixing of asphalt and aggregate • Compaction of sample • Mass of dry sample • Mass under water • Mass saturated surface dry (SSD)**Testing**Obtain mass of dry compacted sample**Testing**Obtain mass of specimen at SSD**Calculations**• Gmb = A / ( B - C ) Where: A = mass of dry sample B = mass of SSD sample C = mass of sample under water**Mass agg. and AC**Vol. agg. and AC Gmm = Maximum Specific Gravity • Loose (uncompacted) mixture**Testing**• Mixing of asphalt and aggregate • Mass in air • Mass under water**Testing**Loose Mix at Room Temperature**Testing**Residual Manometer Metal Bowl with Lid Vacuum Pump Shaker Table**Calculations**• Gmm = A / ( A - C ) Where: A = mass of dry sample C = mass of sample under water**Gmb**Gmm Air voids = ( 1 - ) 100 Mass agg + AC Vol. agg, AC, Air Voids Vol. agg, AC Vol. agg, AC, Air Voids = Mass agg + AC Vol. agg, AC Percent Air Voids • Calculated using both specific gravities**Example Calculations**• Air voids: • Gmb = 2.222 • Gmm = 2.423 ( 1 - 2.222 / 2.423 ) 100 = 8.3 %**Surface Voids**Mass, dry Solid Agg. Particle Effective Specific Gravity Gse = Effective Volume Vol. of water-perm. voids not filled with asphalt Absorbed asphalt Effective volume = volume of solid aggregate particle + volume of surface voids not filled with asphalt**100 - Pb**Gse = 100 - Pb Gmm Gb Effective Specific Gravity Gse is an aggregate property**100 - 5**100 - 5 2.535 1.03 Gse = Example Calculations • Mixed with 5 % asphalt cement • Gmm = 2.535 • Gb = 1.03 = 2. 770**Gmb Ps**Gsb VMA = 100 - Voids in Mineral Aggregate VMA is an indication of film thickness on the surface of the aggregate**(2.455) (95)**2.703 VMA = 100 - Example Calculations • Given that Gmb = 2.455, Ps = 95%, and Gsb = 2.703 = 13.7**VMA - Va**VMA VFA = 100 x Voids Filled with Asphalt VFA is the percent of VMA that is filled with asphalt cement**Ma = 0**Mb = Pb MT MT = Mb + Ms Mass Relationships Ms = Ps MT**Gse - Gsb**Gsb Gse Pba = 100 ( ) Gb Percent Binder Absorbed Pba is the percent of absorbed asphalt by mass of aggregate**Pba**100 Pbe = Pb - Ps Effective Asphalt Content The effective asphalt content is the total asphalt content minus the percent lost to absorption (based on mass of total mix).**Hot Mix Asphalt (HMA) Volumetric PropertiesUsingPhase**Diagrams**Gmb = 2.329**MASS (g) VOL (cm3 ) air asphalt Gb = 1.015 Pb = 5% by mix absorbed asph 1.000 aggregate Gsb = 2.705 Gse = 2.731**M =**V x G x 1.000 Gmb = 2.329 MASS (g) VOL (cm3 ) Ma = 0 air asphalt Gb = 1.015 Pb = 5% by mix absorbed asph Mm = 1.0 x 2.329 x 1.0 = 2.329 1.000 aggregate Gsb = 2.705 Gse = 2.731**Gmb = 2.329**MASS (g) VOL (cm3 ) 0 air asphalt Gb = 1.015 Pb = 5% by mix Mb = 0.05 x 2.329 = 0.116 absorbed asph 2.329 1.000 aggregate Gsb = 2.705 Gse = 2.731 Ms = 2.329 - 0.116 = 2.213**Vse = 2.213 = 0.810**M 2.731x 1.0 V = Vsb = 2.213 = 0.818 G x 1.000 2.705x 1.0 VOL (cm3 ) MASS (g) 0 air asphalt Gb = 1.015 0.116 absorbed asph 2.329 1.000 aggregate Gsb = 2.705 Gse = 2.731 0.818 2.213 0.810**M**Vb = 0.116 = 0.114 V = 1.015 x 1.0 G x 1.000 VOL (cm3 ) MASS (g) 0 air asphalt Gb = 1.015 0.114 0.116 absorbed asph 0.008 2.329 1.000 aggregate Gsb = 2.705 Gse = 2.731 0.818 0.810 2.213 Vba = 0.818 - 0.810 = 0.008**VOL (cm3 )**MASS (g) 0 0.076 air asphalt Gb = 1.015 0.106 0.114 0.116 absorbed asph 0.008 2.329 1.000 aggregate Gsb = 2.705 Gse = 2.731 0.818 0.810 2.213 Vbe = 0.114 - 0.008 = 0.106 Va = 1.000 - 0.114 - 0.810 = 0.076**M =**V x G x 1.000 VOL (cm3 ) MASS (g) 0 0.076 air asphalt Gb = 1.015 0.106 0.108 0.114 0.116 absorbed asph 0.008 0.008 2.329 1.000 aggregate Gsb = 2.705 Gse = 2.731 0.818 0.810 2.213 Mbe = 0.106 x 1.015 x 1.000 = 0.108 Mba = 0.116 - 0.108 = 0.008**VOL (cm3 )**MASS (g) 0 0.076 air 0.182 asphalt Gb = 1.015 0.106 0.108 0.114 0.116 absorbed asph 0.008 0.008 2.329 1.000 aggregate Gsb = 2.705 Gse = 2.731 0.818 0.810 2.213 Air Voids = 0.076 x 100 = 7.6 % VMA = Vbe + Va = ( 0.106 + 0.076 ) x 100 = 18.2 %**VOL (cm3 )**MASS (g) 0 0.076 air 0.182 asphalt Gb = 1.015 0.106 0.108 0.114 0.116 absorbed asph 0.008 0.008 2.329 1.000 aggregate Gsb = 2.705 Gse = 2.731 0.818 0.810 2.213 Air Voids = 7.6 % VMA = 18.2 % VFA = ( 0.106 / 0.182 ) x 100 = 58.2 %**VOL (cm3 )**MASS (g) 0 0.076 air 0.182 asphalt Gb = 1.015 0.106 0.108 0.114 0.116 absorbed asph 0.008 0.008 2.329 1.000 aggregate Gsb = 2.705 Gse = 2.731 0.818 0.810 2.213 Air Voids = 7.6 % Eff. Asp. Cont. = ( 0.108 / 2.329 ) x 100 = 4.6 % VMA = 18.2 % VFA = 58.2 %**VOL (cm3 )**MASS (g) 0 0.076 air 0.182 asphalt Gb = 1.015 0.106 0.108 0.114 0.116 absorbed asph 0.008 0.008 2.329 1.000 aggregate Gsb = 2.705 Gse = 2.731 0.818 0.810 2.213 Air Voids = 7.6% Effective Asphalt Content = 4.6% VMA = 18.2 %Abs. Asph. Cont. = ( 0.008 / 2.213 ) x 100 = 0.4% VFA = 58.2 %**1.000 - 0.076**1.000 VOL (cm3 ) MASS (g) 0 0.076 air 0.182 asphalt Gb = 1.015 0.106 0.108 0.114 0.116 absorbed asph 0.008 0.008 2.329 1.000 aggregate Gsb = 2.705 Gse = 2.731 0.818 0.810 2.213 Air Voids = 7.6% Max Theo Sp Grav = 2.329 = 2.521 VMA = 18.2 % VFA = 58.2 %**VOL (cm3 )**MASS (g) 0 0.076 air 0.182 asphalt Gb = 1.015 0.106 0.108 0.114 0.116 absorbed asph 0.008 0.008 2.329 1.000 aggregate Gsb = 2.705 Gse = 2.731 0.818 0.810 2.213 Air Voids = 7.6% Effective Asphalt Content = 4.6% VMA = 18.2 % Absorbed Asphalt Content = 0.4% VFA = 58.2 % Max Theo Sp Grav = 2.521